# Spectral Investigation of a 2-Dimensional Photonic …essay.utwente.nl/645/1/scriptie_Hagen.pdf ·...

date post

31-Aug-2018Category

## Documents

view

213download

0

Embed Size (px)

### Transcript of Spectral Investigation of a 2-Dimensional Photonic …essay.utwente.nl/645/1/scriptie_Hagen.pdf ·...

R.A.J. Hagen

Spectral Investigation of a

2-Dimensional Photonic Crystal

Slab for mid-Infrared Radiation

University of Twente

Laser Physics and Nonlinear Optics

Faculty of Science and Technology & MESA+ Research Institute

Enschede, September 7, 2007

Graduation Committee:

prof. dr. K.-J. Boller

dr. P. Gro

dr. P.J.M. van der Slot

dr. H.J.W.M. Hoekstra

Abstract

This thesis presents spectral investigations of a two-dimensional (2D) photonic crystal(PhC) which has an exceptional large surface (100mm2). The 2D PhC investigated is madefrom Silicon and was available for fabrication with a novel Laser Interference Lithogra-phy (LIL) technique, where the main design purpose was to provide a modified dispersionfor photon energies of less than half of the electronic band gap of silicon. Here we presentby angular dependent infrared reflectivity and transmission spectra of these crystals asobtained in experiments. Resonance features are observed in polarized reflectivity andtransmission spectra in the near and mid-infrared, which arise from coupling of radiationto PhC leaky modes. We determine the quality factor of the experimentally observed fea-tures and comparing them with upper limit as calculated for the modes supported by ourstructure. This comparison provides the first information on the crystal quality obtainedby the named LIL fabrication.

Contents

1 Introduction 1

2 Theory of Photonic Crystals 3

2.1 Maxwell Equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4

2.2 Dispersion Relation of a 1D PhC . . . . . . . . . . . . . . . . . . . . . . . . 6

2.3 A 2D Photonic Crystal Slab . . . . . . . . . . . . . . . . . . . . . . . . . . . 6

2.4 Influences on the Dispersion Curves . . . . . . . . . . . . . . . . . . . . . . 9

2.5 Quality Factor & Losses . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 11

2.6 Coupling via Vertical Incidence . . . . . . . . . . . . . . . . . . . . . . . . . 12

2.7 Fano Resonances . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 15

3 Computational Modeling Tools 17

3.1 RSoft DiffractMOD . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 17

3.2 MIT Photonic-Bands . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 19

3.3 MIT Electromagnetic Equation Propagation . . . . . . . . . . . . . . . . . . 20

4 LIL-Fabrication of 2D Silicon Photonic Crystals 21

4.1 Design of the 2D PhC . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 22

4.2 Fabrication of the 2D PhC with LIL . . . . . . . . . . . . . . . . . . . . . . 22

5 Transmission Experiment 25

5.1 Set-up for Investigation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 25

5.2 Experimental Transmission Results . . . . . . . . . . . . . . . . . . . . . . . 26

i

Contents

5.3 Simulation Transmission Spectrum . . . . . . . . . . . . . . . . . . . . . . . 27

5.4 Calculation of Expected Intrinsic Leaky Modes Q-factors . . . . . . . . . . 28

6 Reflection Experiment 31

6.1 Principle of Investigation . . . . . . . . . . . . . . . . . . . . . . . . . . . . 31

6.2 Set-up for Investigation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 33

6.3 Experimental Reflectivity Results . . . . . . . . . . . . . . . . . . . . . . . . 34

6.4 Experimentally Extracted Q-factors . . . . . . . . . . . . . . . . . . . . . . 35

6.5 Results and Comparison with Theory . . . . . . . . . . . . . . . . . . . . . 37

7 Conclusions 39

Acknowledgements 41

Bibliography 43

Appendix A: Two-color Characterization of a 2D Photonic Crystal I

ii

Chapter 1

Introduction

The investigation of third-order nonlinear effects in photonic crystals (PhCs) is of highinterest, as these effects might enable an improved temporal and spectral control of prop-agating light for the purpose of integrated optical devices, such as for optical switching.A switching on the femtosecond time scale can principally be achieved with the real-part(refractive index part) of the third order response, which is called the optical Kerr-effect orthe intensity-dependent refractive index. The observation of these effects is hampered bylinear absorption and other losses, such as arising from imperfections from the fabricationprocess. A more fundamental obstacle for fast (fs) switching is, however, the imaginarypart of the third-order response, called two-photon absorption. When two-photon ab-sorption is allowed, i.e., if the sum-energy of two photons is larger than the electronicbandgap, this would excite population into the conduction band. Once excited, this popu-lation would decay rather slowly, with intra-band lifetimes in the ps range, and with up tons inter-band lifetimes, which would limit the speed of optical switching accordingly. Inorder to avoid such two-photon absorption we investigate a special PhC with a relativelylarge spatial period of refractive index modulation. This should shift stop bands into themid-infrared (MIR), where two-photon absorption is suppressed due to the lack of photonenergy. As preparation for later nonlinear studies, the large period enables to characterizethe crystal in the near infrared (NIR), at half of the target (MIR) wavelength, where wecarried out characterizing reflectivity and transmission measurements. This characteri-zation and a comparison with theoretical models provides valuable information on thelinear optical properties of the fabricated crystals which complements a technically morechallenging characterization in the MIR.

Several studies on how resonant guiding in 2D photonic crystal appears in reflection [17] and transmission [8] spectra were reported before. However, the recent demonstrationof a novel type of laser interference lithography (LIL) has made it possible to fabricatelarge area 2D PhCs also from Silicon and for MIR radiation, while optical studies of thequality of these crystals are lacking so far. In this thesis we demonstrate that resonances

1

Chapter 1. Introduction

can be observed in reflection and transmission spectra and we determine the quality ofthe with LIL fabricated MIR PhCs.

In the first chapter we review the theoretical background necessary to understand theexperimental results obtained (Chapter 2). In Chapter 3, a brief description of theoreticalmodeling tools for the calculation of transmission and reflection spectra of the crystal aregiven. In Chapter 4, the fabrication technique which has been used to make our crystalis explained. Then, the experimental results in transmission (Chapter 5) and in reflection(Chapter 6) are analyzed. Finally, in Chapter 7 conclusions are drawn about the qualityof a large area 2D Silicon PhC slab fabricated with LIL.

2

Chapter 2

Theory of Photonic Crystals

Photonic crystals (PhC) are composites of materials with different refractive indices, wherethe materials are arranged in a spatially alternating manner such that the resulting modu-lation period of the refractive index is in the order of the wavelength [9]. Figure 2.1 showsa schematic illustration. On the left a one-dimensional (1D) PhC is illustrated, whichconsists of parallel layers of two different materials with indices n1 and n2 and thicknessa/2. The layers with n1 and n2, are repeated, which results in a superlattice with pe-riod a. To obtain a two-dimensional (2D) PhC, one could think of the 1D crystal cutperpendicular to the layers with every other slice shifted by a/2 as is shown in the middleof Fig. 2.1. Analogously, by slicing the 2D PhC in the horizontal direction, shifting bya/2, one obtains a three-dimensional (3D) PhC with a periodicity of refractive materialalong all directions as illustrated on the right of Fig. 2.1.

Figure 2.1: Schematic illustration of a 1D-, 2D- and 3D-dimensional photonic crystal.

With such structure, the propagation of light in PhCs becomes strongly modified,which can qualitatively be understood as follows. For example, a 1D PhC can be seenas Bragg-reflection in a multi-layer mirror. Propagating light is repeatedly redirected byFresnel-reflection at the material interfaces. Depending on the optical path length differ-ence, which is given by the period a and the refractive index of the layers, the reflectionscan interfere constructively and destructively, such that light with certain frequencies isforbidden to propagate as in a highly reflective multi-layer mirror.

3

2.1 Maxwell Equations Chapter 2. Theory of Photonic Crystals

For 2D and 3D crystals the situation is considerably more complicated because herethe redirection of propagating light occurs via diffraction into two and three dimensions,respectively, which also depends on the polarization of the light. Furthermore, the shapeof the material boundaries is usually not cubic (as in the right hand side of Fig. 2.1) suchthat, generally, the theoretical modeling of light propagation in PhCs requires numericalmeans.

As a basic illustration on how such modeling can be performed we first present in thefollowing a model for the simple case of a 1D PhC. Thereafter, this model is expanded toinclude the case of a 2D PhC, in order to describe the crystal used in the experiments.

2.1 Maxwell Equations

A standard way to describe the propagation of light in photonic crystals is based on themacroscopic Maxwell equations (Eq. 2.1), which were introduced by James Clerk Maxwellin 1864. Here E and H are the macroscopic electric and magnetic fields, respectively. Dand B are the displacement and magnetic induction fields, and f and Jf are the freecharges and free currents, respectively.

B = 0 E + Bt

= 0

D = f HDt

= Jf

(2.1)

The type of PhC used in the experiments described in this work does not contain anyinternal light sources, thus f = 0 and Jf = 0. The Maxwell equations are used todescribe the behaviour of electric and magnetic fields in material in general. To simplifythe Maxwell equations for the case of photonic crystals four simplifications can be applied.

First, it is assumed that the PhC is subjected only to weak radiation field strengths,such that the induced polarization of the medium remains proportional to the electricfield of the light. Second, it is assumed that the dielectric constant at position r doesnot depend on the light frequency , so (r, ) reduces to (r). The third assumptionis that the crystal is macroscopic and isotropic in the sense that, at bulk level, it canbe described via an average refractive index, which is only dependent on the directionand polarization, with which the light travels. With these assumptions, one obtains thatD(r) = 0(r)E(r) and B(r) = 0(r)H(r), where 0 8.854 1012 Farad/m is thevacuum permittivity and 0 = 4 107 Henry/m is the vacuum permeability. Finally,we consider only low-loss (transparent) dielectrics, which means that (r) is purely real.

4

Chapter 2. Theory of Photonic Crystals 2.1 Maxwell Equations

When taking these simplifications into account, Eqs. 2.1 reduces to a set of equa-tions [9],

H(r, t) = 0 E(r, t) + 0H(r, t)

t= 0

[(r)E(r, t)] = 0 H(r, t) 0(r)E(r, t)

t= 0

(2.2)

where, in general, E and H are still complicated functions of both space and time. How-ever, since the Maxwell equations are linear, the time dependence can be separated outby expanding the field into a set of harmonic modes (Fourier expansion as a function ofthe light frequency ). To achieve this, each of these modes H(r, t) and E(r, t) can bewritten as a space-dependent amplitude with a harmonic time dependence

H(r, t) = H(r)eit

E(r, t) = E(r)eit.

(2.3)

Inserting Eqs. 2.3 into Eqs. 2.2 yields a new set of equations which are no longer a functionof time but, instead, scale with the frequency only as an algebraic factor:

H(r) = 0 E(r) i0H(r) = 0

[(r)E(r)] = 0 H(r) + i0(r)E(r) = 0(2.4)

The two divergence equations on the left have the physical interpretation that there are nopoint sources or sinks of displacement and magnetic fields in the medium. With this, onecan eliminate E from the two curl equations on the right and derive an equation separatelyfor H(r):

(

1(r)

H(r))

=(

c

)2H(r) (2.5)

This eigenvalue problem is known as the Helmholtz equation. Where c is the speed of lightin vacuum. The solutions of the Helmholtz equation for a given crystal, described by (r),are a set of modes for each given frequency [9]. The Helmholtz equation can be solvedeasily only for homogeneous media, i.e., with (r) = (z) being constant. The solutionsare, e.g., plane wave modes or spherical waves, such as

Hk(r) = H0(r)eikr. (2.6)

In Eq. 2.6, the wavevector k indicates the propagation direction. The dispersion relationof light in a homogeneous medium is a straight line given by

=c|k|, (2.7)

5

2.2 Dispersion Relation of a 1D PhC Chapter 2. Theory of Photonic Crystals

as can be found by inserting Eq. 2.6 into Eq. 2.5.

In the following two section we are going to develop from a homogenous material to aperiodic structure. We will start with the simple case of a 1D structure and continue witha 2D structure.

2.2 Dispersion Relation of a 1D PhC

Figure 2.1 showed an example for a 1D photonic crystal (a multi-layer mirror). This struc-ture consists of parallel layers of two different dielectric materials that varies periodically,(r) = (r a), i.e., with a superlattice of period a. Figure 2.2 displays the solutions ofthe Helmholtz equation for this mirror. The standard, adopted from solid state physics,is to display the frequency n as a function of the wavevector k (in units of [2a ]) and aband label number n in order of increasing frequency, while the frequencies is normalizedto [2ca ]. Figure 2.2 shows that for each k-value the spectrum is discrete with n solutions,i.e., there is more than one dispersion curve. Most noticeable is that the frequency of thesolutions remains within certain intervals or bands, while there are also frequency intervalsor bands for which no k-value satisfies the Helmholtz equation (indicated as grey area).This is why Fig. 2.2 is usually called a band diagram. Frequency bands without a solutionare called a stopband. Light with frequencies inside a stopband are not allowed to propa-gate through the PhC (i.e., the mirror is high reflective for these light frequencies). Thedispersion curves in Fig. 2.2 has extrema at m0.5 (where m is an integer) and is periodicwith the periodicity 2a . The states of light, i.e. the set of eigenvectors H in Eq. 2.5, thatbelong to a particular frequency, possess periodically occurring k-values and are calledBloch modes.

As, obviously, the entire information of the dispersion relation is already containedwithin one period, from k = 0 to /a, it is sufficient and standard to display the dispersionof PhCs only in this interval, which is also called the irreducible Brillouin Zone (iBZ).Fig. 2.2 is instructive because similar dispersion curves, with allowed and stopgaps appearalso in 2D and 3D crystals, although there the k-vector can assume more than a singledirection.

2.3 A 2D Photonic Crystal Slab

Figure 2.3(a) shows a schematic illustration of a two-dimensional photonic crystal wave-guide similar to the one used in the experiments. The crystal is essentially a high refractiveindex (Silicon) slab containing periodically air filled holes in a square pattern, which giveshigh index contrast with regards to the slab material (nSinair = 2.4). Within the figuretwo distinct directions in plane with the slab can be recognized, the direction parallel with

6

Chapter 2. Theory of Photonic Crystals 2.3 A 2D Photonic Crystal Slab

Figure 2.2: Dispersion relation (band diagram) for a 1D PhC. The gray shaded bands indicatesstopgaps where no modes are present.

the x-axis, i.e., along the sides of the square pattern where the index variation period is thesmallest. At an angle of 45 with the former directions, i.e., crossing diagonally throughthe square pattern, the period is largest.

Figure 2.3(b) shows the BZ of the square lattice PhC shown in Fig. 2.3(a). The BZ is aprimitive cell of the reciprocal lattice (or k-space). The reciprocal lattice is the inverse of thereal-space lattice [10]. The points denoted by , X and M are the high symmetry points,with k-vectors k = 0, k = a x and k =

a x +

a y, respectively. The high symmetry

points enclose the gray shaded triangle called the irreducible Brillouin Zone (iBZ). Thehigh symmetry points are special, because every wave with a k-vector extending from to the iBZ gives rise to Bragg-reflected waves. For a large PhC, i.e. many holes, a waveundergoes multiple scattering as it propagates through the crystal, but because of theperiodicity of the crystal the scattering is coherent. The field can propagate through thecrystal in a coherent manner, to produce a standing wave field as a Bloch mode [9, 10].

(a) (b)

Figure 2.3: A 2D PhC waveguide slab. (a) Schematic illustration of a 2D PhC slab with a squarelattice of air holes introduced into a high refractive slab. (b) Brillouin Zone defined in reciprocalspace. The high-symmetry points , X and M enclose the irreducible Brillouin Zone.

7

2.3 A 2D Photonic Crystal Slab Chapter 2. Theory of Photonic Crystals

Figure 2.4 shows the band diagram for the PhC of Fig. 2.3. The band diagram iscalculated as explained in more detail later (Chapter 3.2). The horizontal axis containsin-plane wavevectors along a path connecting the high symmetry points XM . Thisis sufficient to show all maxima and minima of all bands [11].

Figure 2.4: Calculated band diagram of a 2D PhC square lattice slab. The banddiagram iscalculated for a Silicon slab with a thickness of 500nm and with hole radius of 0.36m. ThePhC is suspended in air. The open circles indicate the even modes and the filled circles indicatethe odd modes.

In this representation, the thick black line is called the light line with = ck||, sincethere is confinement confinement by the slab in the third direction. This light line thenrepresents the frequencies for the k-vectors at which modes can leak out of this slabwaveguide. The external radiation is a continuum of states outside the waveguide slaband therefore indicated by the gray shaded region, called the light cone. Often the lightcone is referred to as the background or cladding [12].

The thin lines with circles show the solutions of the Helmholtz equation, Eq. 2.5. Thesolutions are calculated for two cases: for light polarized in the plane of the photonicslab and perpendicular to the plane of the photonic slab. The modes of the dispersionrelation are presented for the two cases as lines with open circles for the so-called evenmodes and lines with filled circles for the odd modes. This labelling of the modes aseven and odd modes, instead of TE and TM modes, respectively, is based on a mirrorsymmetry argument, as follows. If one considers the electric field profiles of modes in athin (smaller then the wavelenght) dielectric slab, then at the symmetry plane (z = 0)fields must be purely TE or TM polarized, which is parallel or perpendicular to the z = 0

8

Chapter 2. Theory of Photonic Crystals 2.4 Influences on the Dispersion Curves

plane, respectively, shown in Figure 2.5. Since the dielectric slab has a certain thickness

Figure 2.5: Thin dielectric slab with a mirror symmetry at z = 0. The labeling of modes that aremostly parallel, i.e. even, with respect to the mirror plane are TE-like, the modes that are mostlyperpendicular, i.e. odd, with respect to the mirror plane are TM-like.

the fields away of the z = 0 plane can no longer be purely TE or TM polarized, becauseof continuity field should be mostly TE-like or TM-like, which are also called even forpolarizations parallel or odd for polarizations perpendicular to z = 0, respectively [12,13].

In-plane with the photonic slab, photonic modes can be completely confined by totalinternal reflection, when all Bragg-scattering is destructive. Those are referred to as guidedmodes. The guided modes are represented in Fig. 2.4 by the thin lines with open andclosed circles that fall entirely under the light line. Theoretically in a perfectly fabricatedstructure, the guided modes possess an infinite lifetime, which means that there is noenergy transfer with external radiation outside the slab. There are also the radiationmodes or leaky modes which posses a finite lifetime, since they loose there energy to thebackground with which they overlap and thus can couple. The leaky modes are representedby the thin lines with open and closed circles that overlap with the light cone.

In Figure 2.4 it can further be seen that there is a band gap in the even modes in thenormalized frequency range 0.300.39, i.e., there is no allowed frequency for any directionor value of the in-plane k-vector. In this range of frequencies no guided even modes existunder the light line. As a consequence even-polarized light cannot propagate here in planewith the slab.

2.4 Influences on the Dispersion Curves

To get a desired band gap or dispersion curves (here in the mid-IR), there are severalparameters that must be chosen properly. This chapter discusses those parameters to givea hint on what there influences are on the dispersion curves or the existence on positionor size of the band gap.

Effects of the slab thicknessThe slab thickness plays an important role in determining whether a photonic crystal

slab has a band gap in its guided modes. Johnson et al. [12] have predicted that the optimalthickness will be on the order of half the two-dimensional gap-bottom wavelength. Thicker

9

2.4 Influences on the Dispersion Curves Chapter 2. Theory of Photonic Crystals

slabs would easily support higher-order modes. These higher-order modes lie slightly abovethe lowest-order mode, preventing any band gap. On the other hand, a slab that is lessthan half this wavelength only provides a weak perturbation on the background dielectricconstant. Although modes will exist, they will lie close to the edge of the light cone andbe only weakly guided and any gap will be small.

Refractive index contrastThe use of a high refractive index slab is twofold [14]. First, a high refractive index

contrast between slab and cladding provides strong field confinement along the verticaldirection (i.e. the extent of the guided modes outside the slab is small) allowing a largefraction of each mode to interact with the photonic crystal. In Figure 2.6(a) it is illustratedhow the refractive index contrast between the PhC slab and its cladding influences the fieldconfinement. Second, a high refractive index contrast is required between the dielectricmaterial and the holes to open a band gap in the horizontal plane. In practice a contrastof at least 2 is required.

Slabs with symmetry-breaking backgroundsIt has been predicted that PhC slabs can be placed on a substrate with only little effect

on the band gap as long the substrate is separated from the PhC slab by a sufficientlythick buffer region [12]. This buffer region must have a refractive index low enough, sothat a large fraction of the light is still confined in the slab to interact with the photoniccrystal slab. This is illustrated in Figure 2.6(b). The wing of the field reaches deeper intothe buffer region where the refractive index contrast is low.

(a) (b)

Figure 2.6: Field confinement by cladding material. (a) Field confinement in vertical directionwith symmetric cladding. (b) Field confinement in vertical direction with asymmetric cladding.

Introduction of periodic array of holes in the slabThe introduction of a periodic array of holes in the slab has the effect that the disper-

sion relation is folding into the first Brillouin Zone, and opening a band gap in the guidedmodes [14]. Another effect of the holes is that it creates an upper frequency cut-off forthe guided modes. Figure 2.4 shows that the guided modes are cut-off at a normalized

10

Chapter 2. Theory of Photonic Crystals 2.5 Quality Factor & Losses

frequency of 0.7 with the named crystal parameters. Modes above the cut-off frequencyBragg-scatter out of the slab into the background. The cut-off frequency is only deter-mined by the lattice geometry of the array of holes. The PhCs as described in Fig. 2.4with a square lattice have a cut-off frequency of 0.7, while PhCs with a triangular latticehave their cut-off frequency at 0.66 [14]. The array of holes also has the effect that theguided modes are somewhat shifted to higher frequencies. One reason for this is that theremoval of high-index material in the holes lowers the average refractive index of the slab.

2.5 Quality Factor & Losses

In Section 2.3 it is mentioned that there is an energy transfer between the leaky modessupported by the photonic crystal slab and the background. This energy transfer onlyoccurs when in-plane wavevectors from the background are equal to that from the leakymodes. Then a fraction of the light couples from the background to the leaky modes andvice versa, energy in a leaky mode gets lost again to the background within a certaindecay time or lifetime, = 1/, where is the decay rate. Thereby the light that leaksout of a mode attains a phase shift relative to the light in the background which gives riseto resonances in reflection or transmission spectra, where the width of these resonancesbecomes narrower with decreasing decay rate . A widely used measure for the decayrate of the energy stored in damped oscillators and, here, in a certain mode is the qualityfactor Q of the associated resonance and is defined as

Q =0

, (2.8)

where 0 is the leaky mode center frequency and the resonance width at half height.Both 0 and can be obtained from experimental spectra measured in transmission andreflection, as is explained in Section 2.7 [15].

Due to its coupling to the background, the Q-factor for a certain leaky mode is prin-cipally finite, and given by the design of the PhC. If this is the only mechanism limitingthe Q-value, namely diffraction produced by the array of holes [16], Q is said to be limitedby the so-called intrinsic losses. If Q is also limited by other losses, such as fabricationimperfections, this is referred to as extrinsic losses.

Intrinsic lossesThe lifetime given by the intrinsic losses can be seen as related to two roughly inde-

pendent physical effects to each of which a separate Q value can be addressed, Q and Q:Light losses by radiating into the vertical direction, into the background, are addressed byQ and light that decays into the slab plane is addressed to Q.

Increasing the mode confinement increases the Q-factor. As modes get more confine-

11

2.6 Coupling via Vertical Incidence Chapter 2. Theory of Photonic Crystals

ment, this eventually dominates over coupling to the leaky modes, resulting in a higherQ-factor. A symmetry-breaking background may cause that the leakage to one side ismore favorable [14].

Q is strongly influenced by the radius of the holes. With decreasing hole radius, Qincreases, since the resonances asymptotically become true guided modes [17].

The physical independence of the described processes associated with Q and Q makeit possible to define a Q-factor as given by [18]:

1Q

=1

Q+

1Q

. (2.9)

In the case of a large PhC, i.e., in the limit of many holes, Q grows exponential withthe number of cavities formed by a hole in the slab, while Q remains roughly fixed. Byadding many holes then Q saturates at Q.

Extrinsic lossesExtrinsic losses originate, e.g., from fabrication imperfections and are in general un-

desired. Typically, with current fabrication techniques, the extrinsic losses are one orderof magnitude higher then the intrinsic losses, and thus have an significant influence onthe Q-factor [19]. This also explains why it is important to experimentally characterizethe actual Q-factor achieved with the particular fabrication method used (here LIL), in-stead of assuming the theoretically expected Q-factor as based only on the crystals designparameters.

There are many types of fabrication errors that can contribute to the extrinsic losses:limited etch depth, roundness of holes, roughness of surfaces or sidewalls [20], taperedsidewalls [21], hole displacements [22] and irregularities regarding the hole size. Howall these loss factors are reinforcing, or, are counteracting each other is very difficult topredict. Some of these loss mechanisms have been studied to more detail, but always forone loss mechanism at a time. In conclusion the extrinsic losses may be better reducedby trying to improve the fabrication method, assisted by an experimental determinationof the Q-values.

2.6 Coupling via Vertical Incidence

In order to couple light into the PhC slab, k-vectors in-plane with the slab are required.Obviously, light incident at normal incidence does not contain those k-vectors. Neverthe-less, coupling is possible due to diffraction at the small holes inside the PhC slab. Anothereffect expected from vertical incidence to the PhC surface is the occurrence of Fabry-Perotinterference, due to Fresnel-reflection from the planar transparent layers the PhC consistof.

12

Chapter 2. Theory of Photonic Crystals 2.6 Coupling via Vertical Incidence

Diffraction of a wave at an apertureTo illustrate the former diffraction coupling, Figure 2.7 shows a sequence of images

for which we calculated the shapes of a plane wave after being transmitted through aper-tures of different sizes. The resulting pattern behind the aperture can be understood viaHuygenss principle as the interference pattern formed by a large number of point sourcesclosely spaced across the width of the aperture. For example, the minima that are visiblebehind the aperture are the result of destructive interference between the various pointsources. In Figure 2.7(a) the aperture has a size that is about five times the wavelength. Itcan be seen that only at the edge of the aperture the overall wave shows some diffractionwhile most of the wave is just passing the aperture, maintaining its propagation direc-tion. In Figure 2.7(b) the aperture is comparable to the wavelength, such that diffractionbecomes stronger. In Figure 2.7(c) the aperture size is approximately as small as thewavelength. In the case the aperture is so small that it acts like a single point source,thus sending out a hemispherical wave in which the amplitude does not vary much withthe emission (diffraction) angle. Correspondingly, a larger fraction light is diffracted closeto a right angle and then propagates with a k-vector in-plane with the obstructing wallcontaining the aperture.

(a) (b) (c)

Figure 2.7: Diffraction of waves passing different apertures [23]. (a) Aperture size is largerthan wavelength. (b) Aperture size is comparable to wavelength. (c) Aperture size is smaller thanwavelength.

Fabry-Perot interference by multiple reflectionsTo illustrate the origin of Fabry-Perot fringes, Figure 2.8(a) shows a plane wave (il-

lustrated by rays) that enters a planar transparent layer and undergoes multiple internalFresnel-reflections between the two reflecting surfaces, before it is (partially) transmitted.Figure 2.8(b) shows the corresponding Fabry-Perot interference fringes calculated in thetransmission as a function of the wavelength as expressed in Eq. 2.11. The interferenceis maximally constructive when the optical path length between the transmitted partialwaves attain a phase difference that is an integer multiple of the wavelength. Fromgeometrical considerations using Fig. 2.8(a) this phase difference is a function of incident

13

2.6 Coupling via Vertical Incidence Chapter 2. Theory of Photonic Crystals

(a) (b)

Figure 2.8: Fabry-Perot interference fringes from one layer. (a) Light enters a planar transparentlayer that undergoes multiple internal reflections. (b) Fabry-Perot interference fringes calculatedwith Eq. 2.11 for incident angle = 0, reflection coefficient r = 0.3, refractive index n = 3.4 andlayer thickness l = 2 m.

angle , refractive index n and thickness l of the layer:

=(

2

)2nl cos(). (2.10)

Because, at a single layer, the Fresnel-reflection coefficient r is the same on both sur-faces, the transmission Ttot can be calculated with Eq. 2.11, which describes the case thatabsorption and scattering losses can be neglected, i.e., Rtot = 1 Ttot.

Ttot =(1 r)2

1 + r2 2r cos(). (2.11)

Equation 2.11 shows that the distance between the fringes in Fig. 2.8(b) becomessmaller when the light propagates through effectively more material which creates a longeroptical path length difference. This can be realized by increasing the layer thickness, theangle of incident or choosing a material with a higher refractive index. A change to therefractive index, however, also increases the reflection coefficients between the interfaces,which will decrease the spectral bandwidth of the transmission peaks.

We note that Fig. 2.8 describes only the basic principle of how a simple layer structure(here a single layer) creates Fabry-Perot fringes in transmission. In the PhCs used inour experiments there are actually three layers (500nm Silicon and 3m SiO2 on 522mSilicon) which is, however, included in the theoretical calculations.

14

Chapter 2. Theory of Photonic Crystals 2.7 Fano Resonances

It should be pointed out that layers with m-range thicknesses lead to a rather slowvariation with wavelength, to broad features that appear like a slow variation of somebackground spectra. An even thinner layer, say the 500nm top layer of our sample usedin the experiments leads to even slower variations of the background.

In contrast to the slow variation of the background spectra, the spectra in reflectionand transmission also contains sharp resonances superimposed on the background spectra.These sharp resonances are formed by a second process that takes place, explained in thenext section.

2.7 Fano Resonances

The sharp resonances which we observed in reflection and transmission spectra on a PhCexhibit all the properties of dispersive line shapes as described by Fano in 1961 [24].These sharp resonances are of major interest, because it shows how well LIL-fabricationis performed to create photonic slab waveguides.

It shows that the sharp spectral features are actually formed by two independentprocesses. The first process, direct reflection or transmission modified slowly by Fabry-Perot interference, is of minor interest. The second process, is excitation of resonances(states, modes) of the photonic crystal, is of major interest, because in this process partof the light is first coupled to the PhC slab and via second diffraction the light leaves thePhC partly in the direction of the directly reflected or transmitted beam and interfereswith it. From this resonances appear in the transmission spectrum. It is thus necessaryto separate these two transmission processes from each other, i.e., to extract from thespectra the positions and widths of the second (PhCmoderelated) spectral resonances.This can be achieved by Fano-fits to the measured resonances which yield the 0 and thewidth (, q) independently from the direct reflection or transmission process.

Although the original Fano-function was a description of such asymmetric resonancesas based on excitation spectra of inelastic scattering of electrons on Helium atoms, it canalso be applied to reflection and transmission spectra on PhC, due to the parallels betweenthe Helium experiment and the experiments in this work. In the Helium experimentelectrons either pass the Helium unmodified or excite the Helium atoms to its discreetatomic resonant states. In our experiments the incoming (external) light has the role ofthe electrons and the discreet atomic resonant states can be seen as the PhC leaky modes.

15

2.7 Fano Resonances Chapter 2. Theory of Photonic Crystals

Fano resonances in the case of photons coupling to the PhC leaky modes is given by:

f() = f0

[1 +

q2 1 + 4q( 0)/1 + 4( 0)2/2

]. (2.12)

Here, f0 is the oscillation strength. Figure 2.9 shows how the coupling parameter q de-termines the shape of the Fano function. A q of 0 means that the energy leaks into aphotonic crystal mode without a phase shift, resulting in a symmetric dip in the intensity.For higher q values the resonances become asymmetric and the exact centre frequency 0of 200THz is less obvious in the figures.

Figure 2.9: Fano lineshapes for = 0.3THz, = 200THz and different q values. From left toright q value is 0.0, 0.3, 0.6 and 1.0 respectively.

16

Chapter 3

Computational Modeling Tools

Due to the great complexity encountered with photonic crystals, there are numerous dif-ferent approaches to predict their properties. Each of these approaches has its own capa-bilities and limitations. Depending on the goal of the analysis and design of the PhC, themost convenient tool is thus to be selected [18,19].

Since a full treatment about all available methods goes far beyond the scope of thisthesis, we restrict ourself to the three models used in our evaluation of PhCs, namely:The rigorous coupled wave analysis (RCWA), a variation method and a finite differencetime-domain (FDTD) method. Each of these methods is implemented as a computeralgorithm with its own software known as DiffractMOD, MPB and Meep, respectively. Inthis chapter we give for each of these software tools a short description, together with itscapabilities and its limitations. Something that all of these tools have in common is thatthey divide space in repeating computational cells. Such a computational cell is then filledwith a distribution of refractive index materials, to represent one period of the PhC. Thisdata is inserted into equations derived from the Maxwell equations (Eq. 2.1) and evaluatedby the simulation tool.

3.1 RSoft DiffractMOD

DiffractMOD is a commercially available simulation tool developed by RSoft Design Group,Inc. With DiffractMOD a wide range of scattering situations on structures can be ana-lyzed. It solves full vectorial versions of the Maxwell equations by implementing therigorous coupled wave analysis (RCWA) method [25]. The software tool calculates re-flection and transmission diffraction efficiencies at any diffraction order in the form of areflection or transmission spectrum.

In the RCWA method a computational cell can have any arbitrary geometry on whichthe simulation is performed. Within a computational cell a refractive index distribution is

17

3.1 RSoft DiffractMOD Chapter 3. Computational Modeling Tools

specified that represents the photonic crystal structure. At the surfaces of the computa-tional cell, certain boundary conditions are to be applied, because there is no informationfrom outside the cells available. A common boundary condition is the so-called perfectlymatching layer (PML). This represents a (non-physical) material that, in theory, absorbswaves without any reflection, at all frequencies and angles of incidence [26]. Materials andwaves adjacent a PML can be interpreted as ongoing at the outside of the computationalcell. Surfaces of the computation cell to which no PML is added, are assumed to berepeated by a copy of the computational cell.

Figure 3.1(a) is a graphical presentation of a computational cell filled with an indexdistribution as given by correspondingly placed materials and on bottom and top end ofthe cell a PML. There are no PMLs added in the horizontal directions, because the indexmaterials are considered to repeat periodically and infinetely in the horizontal plane. Insidethe computational cell of Fig. 3.1(a) the stack of materials represent a photonic crystal slabwith an asymmetric cladding (index and thickness of cladding 1 different from cladding2). The hole being centered in the square xy-plane makes this a square lattice photoniccrystal that is periodic with the size of the computational cell.

(a) (b)

Figure 3.1: (a) Computational cell for a 2D square lattice PhC structure. (b) Fourier expansionof refractive index material in xy-plane.

The RWCA method expresses the spatial variations of the refractive index as a Fourierexpansion of the index as found in slices. Figure 3.1(b) illustrates this for the xy-plane.The widths of slices is chosen to model the distribution of the refractive index as closely aspractical with a minimum number of slices. The related input and output fields are com-puted by matching the boundary conditions at every slice. A limitation of this method isthat the Fourier expansion introduces a discretization to the distribution of the refractiveindex, which leads to a staircase effect, as shown in Fig. 3.1(a). The RWCA method incombination with PMLs and the named staircase approximation lead to complex eigen-value problems. For these reasons RWCA is a method that is sensitive to convergenceproblems [19,27].

18

Chapter 3. Computational Modeling Tools 3.2 MIT Photonic-Bands

3.2 MIT Photonic-Bands

MIT Photonic-Bands (MPB) is a freely available software package released under theGPL license at Massachusetts Institute of Technology (MIT). MPB directly computeseigenstates and eigenvalues of the Maxwell equations in the frequency domain [28]. MPBimplements a variation method, which takes a Fourier transform over an infinite repe-tition of the computational cell as in Fig. 3.1(a), into all directions to avoid any stepdiscontinuities, except where PMLs are placed.

Figure 3.2 illustrates that the repetition of computational cells introduces a new periodin vertical direction. As a consequence, MPB can only calculate the guided modes at highprecision, since those are strong localized within the PhC slab. Leaky modes, however,which are not strongly guided, remain therefore primarily dependent on the period intro-duced in vertical direction. The coupling of leaky modes affecting the guided modes canbe reduced to a negligible level by choosing a computational cell that is long in verticaldirection, such that the newly introduced periodicity is large. Typically, a few times thelattice constants is sufficient for the height of the computational cell.

Figure 3.2: Repetition of a computational cell in vertical direction introduces a new periodicity.

The strength of MPB is that it can calculate band structures and eigenstates veryaccurately. MPB finds every eigenstate, and even modes with closely spaced frequenciesappear as individual modes. The results improves with every new computational iteration.A disadvantage of the frequency-domain methods is that calculations always start at thelowest-frequency eigenstates, up to the desired one [29].

19

3.3 MIT Electromagnetic Equation Propagation Chapter 3. Computational Modeling Tools

3.3 MIT Electromagnetic Equation Propagation

MIT Electromagnetic Equation Propagation (Meep) is a freely available software packagereleased under the GPL license at Massachusetts Institute of Technology (MIT). Meep im-plements the finite difference time-domain (FDTD) method where the propagation of fieldsis calculated directly as a function of space and time, according to Maxwells equations.However, for this it is required to specify, within a computational cell, light sources andflux planes (that model detectors), to generate light and follow its propagation throughthe structure. The electromagnetic fields are evolved in discreet time steps [18] after thecomputational cell has been divided in a discreet spatial grid.

Meep can analyze a versatility of electromagnetic situations. The resulting field pat-terns can be visualized and analyzed in pictures or movies for given light sources. Trans-mission and reflection spectra can be computed at each frequency separately, or for a broadspectrum via a single computation followed by a Fourier-transformation of as the responseto a short pulse emitted by the source. Meep can also calculate the decay time of cavityresonant modes and determine its quality factor Q. In contrast with MPB, Meep can havedifficulties resolving modes that are closely-spaced in frequencies but Meep calculates allfrequency modes at the same time, not consecutively.

20

Chapter 4

LIL-Fabrication of 2D Silicon

Photonic Crystals

For the purpose of complete temporal and spectral control of propagating light in theMIR wavelength range, a 2D PhC has been fabricated. Depending on the requirements onPhCs there are several techniques available. A flexible approach to create PhCs with anyarbitrary shape is focused ion beam lithography [30] and electron beam lithography [31].With these techniques holes are written in a sequential manner, which is a strong limita-tion when large structures are to be fabricated. Other techniques which are less flexible,but provide excellent long-range periodicity are x-ray lithography [32], deep UV lithog-raphy [33] and laser interference lithography (LIL) [34]. The latter method is chosen asfabrication method for our sample to produce a PhC with an exceptionally large surface(100mm2), compared to e-beam or ion-beam-fabricated samples that usually are restrictedto areas of about 100 100m. LIL provides an excellent periodicity over a large surfacewithout any stitching errors. The large surface of our sample is a significant advantage forreflection and transmission experiments. The reason is that, particularly in the mid-IR,the light flux even from powerful sources of incandescent light (e.g. lamps) is extremelylow after spatial and spectral filtering. With large area PhCs spatial filtering can be muchrelaxed, which yields a much higher light flux though the sample. In summary, the largearea of our LIL-fabricated crystals enables a simple setup and short measurement times,which both contribute to a high signal-to-noise ratio.

This chapter describes the design of our PhC and gives a brief overview on the LILfabrication method used. A detailed description of the fabrication of our sample is pre-sented in [35]. This chapter finishes with a description of our sample as it is used in theexperiments presented in this work.

21

4.1 Design of the 2D PhC Chapter 4. LIL-Fabrication of 2D Silicon Photonic Crystals

4.1 Design of the 2D PhC

Figure 4.1 displays a schematic illustration of the intended design for the PhC. As a basisfor the PhC a Silicononinsulator (SOI) wafer [36] is chosen. Silicon is chosen becauseof its transparency for infra-red radiation, its high refractive index and because it is wellknown in material science. The wafer consists of three layers: a mono crystalline Si toplayer, with a thickness of 0.5m and a refractive index of n 3.4. The top layer is goingto host the holes and serves as the PhC slab. Underneath the top layer is a 3m thickSiO2 buffer layer with a low refractive index of n 1.4. The bottom layer is a 522mthick Si substrate with a refractive index of n 3.4 to mechanically support the PhCslab with its buffer layer. The holes in the top layer are intended to obtain a radius of

Figure 4.1: Schematic illustration of the 2D PhC as designed for the experiments presented inthis work.

0.4m with square patterned periodicity of 1m. This design has an expected band gaparound a normalized frequency of 0.4 ( 2.5m) for TE polarized radiation. Note that,at this wavelength, the photon energy is less than half of the electronic band gap of Siliconwhich would, in later experiments, allow to study Kerr-induced switching effects withoutthe slowing effect of two-photon absorption.

4.2 Fabrication of the 2D PhC with LIL

In order to start with the LIL process the surface of the SOI wafer is first coated with anegative photoresist that responds to UV light, which later is going to serve as a maskwith holes through which various etching processes are performed to transfer the patterninto the top layer of the wafer.

For the LIL exposure two continuous-wave UV laser beams with a large (3cm2) cross-section are superimposed to form a well controlled optical interference grating on the

22

Chapter 4. LIL-Fabrication of 2D Silicon Photonic Crystals 4.2 Fabrication of the 2D PhC with LIL

surface of the photoresist. With a first exposure (held under the response threshold of theresist) a 1m periodic striped pattern is irradiating the photoresist. A second exposureis followed with the same interference pattern however, with the wafer rotated by 90

around its surface normal. As a result of the two exposures, which together surpass thethreshold of the resist, a square pattern is written into the photoresist. Heating the waferto a temperature of 125C for 120s leads to the development of the photoresist. Theother areas are removed by chemicals, resulting in a mask of photoresist on the top layer.Various etching processes are followed afterwards to transfer the pattern into the Si toplayer.

The resulting PhC is displayed in the SEM micrograph of Figure 4.2. The micrographshows the edge of the PhC to enable a view also inside some of the holes. The micrographshows that the depth of the holes is seen to be equal to the thickness of the Si top layer,which means that the etching process is stopped, before it would have go into the SiO2buffer layer. A closer look depicted in the upper right corner of the SEM micrograph showsa sub-micron structure inside the holes and on the walls due to fabrication imperfections.These sub-micron structures causes light to scatter out the PhC during experiments, whichattribute to the PhC extrinsic losses (see Section 2.5). And so will do any other unwantedirregularities from the fabrication process like, for instance, dust and cracks.

Figure 4.2: SEM micrograph of the with LIL fabricated PhC. The magnified image in the upperright corner shows a sub-micron structure that originate from fabrication imperfections.

The described fabrication delivered a 2D PhC with a large surface of 100mm2. Deter-mined from SEM images the holes have approximately the intended radius of 0.4m. Themeasured polydispersity is less than 6% placed in a 1m periodic square pattern. Con-sidering that the crystal is immured in air with a refractive index of n = 1 the refractiveindex contrast is n = 2.4. The buffer layer and substrate remain unchanged. Table 4.1summarizes the PhC structure parameters.

23

4.2 Fabrication of the 2D PhC with LIL Chapter 4. LIL-Fabrication of 2D Silicon Photonic Crystals

Table 4.1: PhC Structure Parameters

PhC surface dimension 10 10mmhole radius 0.4m

lattice periodicity 1.m

PhC slab thickness 0.5mcladding thickness 3.0m

substrate thickness 522.m

refractive index nSi 3.4 (PhC slab)refractive index nSiO2 1.4 (cladding)

refractive index nSi 3.4 (substrate)

The described PhC, particular due to its large surface, is very suitable for the experi-ments described in the next two chapters, where light is to be coupled into the PhC modesvia the surface of the PhC slab. In the two following chapters, two spectral experiments arepresented. The first is a transmission experiment and the second a reflection experiment.

24

Chapter 5

Transmission Experiment

The transmission experiment that is presented in this chapter has been performed incollaboration with our partners in Germany at the Physikalisch-Technische Bundesanstalt(PTB) in Braunschweig, Department of Spektrometrie und mikrooptische Messtechnik. Inthis experiment the sample of Chapter 4 is placed in a Cary 5E spectrometer to measureits transmittance.

In this experiment the transmission spectrum is recorded as a function of wavelength.The experiment relies on the coupling of external radiation to leaky modes of the photoniccrystal, as has successfully been applied earlier by K.B. Crozier, et al. in 2006 [8], however,with free-standing membranes fabricated with much smaller area (100 100m) with anion-beam technique.

The content of this chapter is organized as follows. First an overview over the exper-imental set-up in Section 5.1 is given. Then, the transmission spectra are presented inSection 5.2. In Section 5.3 the transmission spectra are compared to calculated transmis-sion spectra to obtain the structural parameters for our PhC as seen by infra-red light.These parameters are used in a second calculation (Section 5.4) to predict the upper limitof the quality factors for the crystal leaky modes.

5.1 Set-up for Investigation

The transmission experiment is performed with a Cary 5E spectrometer which is connectedto a computer that records the transmittance as a function of wavelength. The spectrumis recorded over the wavelength range of our interest between 1.1m to 2.4m. In frontof the PhC a linear polarizer is placed to set the polarization.

Since the illumination beam of the spectrometer is diverging a tube is placed in thebeam path to obtain a spot-size of 2.5mm by 1.5mm. Note that small area PhC, such as

25

5.2 Experimental Transmission Results Chapter 5. Transmission Experiment

with an area of 100 100m, would have required to reduce the beam area by anotherfactor of 400. Assuming the standard square root law for shot noise this would haveincreased the measurement time by approximately a factor 20 for the same signal-to-noiseratio. In the far field the beam divergence is 4 in vertical direction and 3.4 in horizontaldirection.

The sample is placed vertical with respect to the direction of beam propagation, in amount that can rotate the sample around its surface normal. Behind the sample there isa hole in the mount so that the transmitted light can reach a detector placed behind thesample.

5.2 Experimental Transmission Results

Figure 5.1 shows the measured transmission spectra as a function of wavelength. Thepolarization of the light is aligned for three angles with regard to the crystals symmetrydirections, namely along the M , X and an intermediary direction. The transmissionis recorded over the wavelength range from 1.1m to 2.4m, displayed on the horizontalaxis. On the vertical axis the spectral transmittance is displayed.

Figure 5.1: Transmission spectra at normal incidence as a function of wavelength. Three mea-surements where performed with linear polarized light aligned along X, M and the intermediarydirection to verify that the spectra are polarization independent.

Within the transmission spectra there are two types of resonances visible: Fabry-Perot fringes and sharper resonances superimposed on them. The occurance of these typeof resonances have been explained qualitatively in Chapter 2.7.

As a guidance for the eye each Fabry-Perot fringe is given its own colored background.

26

Chapter 5. Transmission Experiment 5.3 Simulation Transmission Spectrum

The left side of Fig. 5.1 is not given a background color, since we learned from calcula-tions that at these wavelengths there is a high mode density, which excludes to identifysingle modes within the spectral resolution of the measurements. From this and the smallthickness of the top layer resulting in a wide fringes spacing we can not recognize series ofFabry-Perot fringes in that part of the spectra, as may be suggested by Fig. 2.8.

The high similarity of the three spectra shows that the transmittance is polarizationindependent at normal incident. Something we find remarkable, since the X and Mdirection have different periodicities, 1m and

2m, respectively. A real physical argu-

ment why the spectra must be polarization independent at normal incident, we currentlydont have. In Ref. [37] this polarization independence has also been observed in sim-ulations. And has been found to be due to the 90 rotational symmetry of the squarelattice.

5.3 Simulation Transmission Spectrum

In this section the measured transmission spectra of Figure 5.1 are compared to the trans-mission spectrum calculated with the RCWA model implemented in DiffractMOD (seeSection 3.1). In order to get a best fit there are eight structure parameters to vary. Ta-ble 5.1 lists these eight parameters as obtained from a best fit. It should be noted that

Table 5.1: DiffractMOD Simulation Structure Parameters

incident angle 3.0

hole radius 0.38m

PhC slab thickness 0.55mcladding thickness 2.80m

substrate thickness 0.01m

refractive index nSi 3.45 (PhC slab)refractive index nSiO2 1.44 (cladding)

refractive index nSi 3.45 (substrate)

the simulation has been performed with a substrate thickness of 0.01m instead of theactual substrate thickness of 522m. The reason for this is that the simulations run intoa memory error for large computational cells that are required for such thick substrates.With the assumed substrate the reflection coefficient is correct on the claddingsubstrateinterface and by setting the thickness to well below the wavelength the period of corre-sponding Fabry-Perot fringes is strongly increased, far beyond the range accessible in theexperiments. This resembles the situation in the experiments where, within the spectralresolution, the fringes from the thick substrate cannot be identified as well and ratherform a spectrally independent background as well. It is supposed that the influence of

27

5.4 Calculation of Expected Intrinsic Leaky Modes Q-factors Chapter 5. Transmission Experiment

either a 522m or a 0.01m thick substrate does not have a significant influence on theresulting spectra.

In Figure 5.2 a measured transmission spectrum (top) is compared to the calculatedtransmission spectrum (bottom) using the fit parameters of Table 5.1. The figure uses thesame variation of background colors as in Fig. 5.1 to highlight the Fabry-Perot fringes.Most noticeable is the fair agreement between measurement and simulation in width,height and positions of the fringes. With darker colored bands sharp resonances superim-posed on the Fabry-Perot fringes are emphasised that originate from coupling to the PhCleaky modes. Although on comparison between measured and simulated spectra, the sharpresonances do not always exhibit the same shape and position, there is a correspondenceof position with respect to their background Fabry-Perot fringes. Because of this reasonwe feel confident that the values listed in Table 5.1 are suitable to calculate the expectedintrinsic quality factors of leaky modes as described in the next section.

Figure 5.2: Comparison between measured transmission spectrum (top) and simulated transmis-sion spectrum (bottom).

5.4 Calculation of Expected Intrinsic Leaky Modes Q-factors

In order to calculate the intrinsic quality factors for leaky modes with Meep (Section 3.3)a computational cell is specified based on the data in Table 5.1 that where obtained bya fit of the RWCA model to the experimental spectra, except for the substrate thickness.Instead, the Silicon substrate is extended into the lower perfectly matching layer (PML),

28

Chapter 5. Transmission Experiment 5.4 Calculation of Expected Intrinsic Leaky Modes Q-factors

such that the substrate is interpreted as extending beyond the outside of the computationalcell, i.e. the calculation assumes the substrate to be of infinite thickness.

The strategy to calculate leaky mode quality factors is to place a short pulse light source(containing a broad bandwidth) inside the PhC slab, such that modes with frequenciesinside that bandwidth get excited. Once the light source is turned off, light of certainfrequencies remains oscillating inside the structure before, eventually, the oscillations aredamped out. Meep then Fourier-analyzes this superposition of damped oscillation toextract the PhC mode frequencies and their decay rates or, equivalently, the Q-values [18].In order to obtain the quality factors more accurately, we repeated the calculations foreach identified mode frequency, however, with a reduced bandwidth of the light source,centered around each particular mode frequency. The mode frequencies as calculated forTE and TM polarization are listed in Table 5.2 together with their corresponding qualityfactor. The table show that quality factors have values that vary from 60 to 1800 for TE

Table 5.2: Meep Q-Factor CalculationsTE TM

norm. frequency Q-factor norm. frequency Q-factor0.835 262.65 0.945 313.680.820 60.07 0.927 443.720.815 1868.60 0.896 295.510.787 841.53 0.873 255.330.775 260.94 0.847 311.220.750 402.72 0.828 1120.210.744 95.27 0.815 462.960.734 134.43 0.795 606.250.724 62.93 0.779 149.720.715 87.20 0.759 1486.570.708 492.88 0.739 324.180.704 189.21 0.725 95.370.700 245.49 0.719 358.630.651 193.77 0.704 161.140.597 68.84 0.702 139.94

0.658 1536.080.603 273.22

modes, and values of 90 to 1500 for TM modes.

The distribution of the quality factors are shown in the histograms of Figure 5.3, wherethe lhs histogram is for TE polarization and the right histogram is for TM polarization.

29

5.4 Calculation of Expected Intrinsic Leaky Modes Q-factors Chapter 5. Transmission Experiment

Figure 5.3: Quality factor histograms: (a) TE polarization, (b) TM polarization.

30

Chapter 6

Reflection Experiment

In this chapter, reflection experiments are described, as performed at the University ofTwente, Laser Physics and Nonlinear Optics (LPNO) group using a homebuild set-up. Inthis experiment the sample as described in Chapter 4 is characterized.

In Section 6.1 we describe the principle of the experiment is explained, followed byan overview of the experimental set-up in Section 6.2. Then, the reflectivity results arepresented in Section 6.3. In Section 6.4 the reflectivity results are analyzed and the qualityfactor for the PhC leaky modes are extracted.

6.1 Principle of Investigation

The dispersion of leaky modes of the PhCs can be reconstructed based on resonant couplingobserved in reflectivity measurements as a function of wavelength and incidence angle.The technique relies on the coupling of external radiation to leaky modes of the photoniccrystal, and has successfully been applied earlier by V.N. Astratov, et al. in 1998 to thin,ion-beam fabricated membranes of much smaller area [1, 38]. By recording the reflectionspectra for a number of incidence angles along the two symmetry directions X and M ,particular resonances shift in wavelength and dispersion curves of the leaky modes can beconstructed.

Resonant coupling only occurs when the projected wavevector k of the incomingbeam matches the wavevector of the photonic leaky modes. Figure 6.1 displays k asthe projection of the incoming wavevector k along one of the symmetry directions. Thesymmetry directions X and M are selected by mounting the sample on a rotation stagethat can rotate around the sample surface normal. A second rotation stage (not drawnin Fig. 6.1) is required to vary the incident angle . The length of k is a function of the

31

6.1 Principle of Investigation Chapter 6. Reflection Experiment

Figure 6.1: Geometry for reflection experiments. A collimated incidence beam is send under anangle to the photonic crystal. The reflection is measured under an angle . By rotation of thesample, the symmetry directions X and M are selected.

incoming wavelength air in air and the angle of incidence :

k = k sin =2air

sin. (6.1)

Based on the symmetry direction selected, via the relative orientation of the E-field andthe crystal rotation, the incident angle of the light and the wavelength, corresponds toexactly one position inside the light cone of a banddiagram. So, if the symmetry directionand the incident angle are kept constant during one measurement, changing the wavelengthcorresponds to a movement along one of the dotted lines drawn inside the banddiagram ofFigure 6.2. Each dotted line correspond to an angle . Fig. 6.2(a,b) gives the X and theM direction of the banddiagram, respectively. Depending on the alignment of the lightpolarization perpendicular or parallel to the plane of reflection, only even or odd modesare excited, respectively. For simplicity only the odd modes are displayed in the figure. Byscanning the wavelength, one scans the k||-vectors from the background which is in-planewith the PhC slab, as given by Eq. 6.1. Energy transfer to the PhC leaky modes and thusresonances in the reflectivity only occur when the k||-vector equals the PhC leaky modewavevector. Thus by identifying the frequencies of resonances and their change with theangle of incidence, one can sample the bandstructure of leaky modes.

In order to select any particular position in the light cone one needs a set-up with thepossibility to illuminate the sample under known angles and and with a proper beamshaping to provide a sufficient angular resolution. The next section describes our set-upin order to fulfill these criteria.

32

Chapter 6. Reflection Experiment 6.2 Set-up for Investigation

(a) (b)

Figure 6.2: X and M direction of a banddiagram. The dotted lines correspond to the angleof incidence .

6.2 Set-up for Investigation

For the precision required single reflection resonances and their angular dependence itis necessary to optimize both the spectral and spatial resolution of the set-up. A goodspatial (k-vector) resolution is needed to accurate select a position inside the light cone.The spectral (frequency) resolution will mainly limit the contrast of the resonances in thereflection spectra.

Figure 6.3 displays a schematic illustration of the set-up used. A 250W quartz tungsten-halogen (QTH) radiation source (Oriel 66995) driven by a stabilized current supply (Oriel 69931)generates a broad spectrum in the infra-red. The light is focused with a 150mm focal

Figure 6.3: Schematic illustration of a home build out of plane reflectivity set-up.

33

6.3 Experimental Reflectivity Results Chapter 6. Reflection Experiment

length plane convex lens (L1) into a monochromator (Hilger and Watts) that selects thedesired wavelengths between 1.1m to 1.9m. The lens and the monochromator are setto the same acceptance angle for efficient throughput. The monochromator has a gratingof 750 lines/mm and entrance/exit slits widths set to 0.75mm, which gives a spectral res-olution of 3.5nm. Light leaving the monochromator is focused by a second lens (L2) to anadjustable diaphragm and travels through a high-pass filter which blocks all wavelengthsbelow 1m that leave the monochromator via higher order diffraction. With an IR polar-izer (Thorlabs LPNIR050) the TE or TM field is set either parallel or perpendicular tothe plane of reflection. The following adjustable diaphragm makes part of a diaphragmlensdiaphragmsample configuration such that the image of the first diaphragm is relayedonto the sample. The diaphragms limit the beam spotsize to 3mm at the center of thesample. The diaphragmlensdiaphragmsample configuration yields a full beam diver-gence of about = 1. The sample is placed in a mount that enables rotation alongtwo axis, such that and can be varied as shown in Figure 6.1. The sample itself isplaced at the center of the two required rotation stages such that always the same areaof the sample is illuminated. About 30% of the light is reflected at the Si surface of thesample. With lens L3 the reflected light is collected and projected on a lead sulfide (PbS)detector (Newport 70323). Since the set-up is optimized for its resolution, most light islost along the set-up (monochromator and diaphragms) which makes the detectability ofthe light more difficult. To improve the signaltonoise ratio (S/N) the detector is used incombination with an optical chopper and a lock-in amplifier (Princeton Applied ResearchCorp., model 129A) this way nano Watt power levels could be detected with a typical S/Nof better than 10.

6.3 Experimental Reflectivity Results

Figure 6.4 shows the measured reflectivity spectra as a function of wavelength for thetwo symmetry directions X and M . In Figure 6.4(a) and Figure 6.4(b) the light isTE polarized, i.e. the electric field is set perpendicular to the plane of reflection. InFigure 6.4(c) and Figure 6.4(d) the light is TM polarized, i.e. the electric field is setparallel to the plane of reflection. The reflectivity is taken in the wavelength range between1.1m to 1.9m in steps of 10nm, displayed on the horizontal axis. After dividing outthe spectrum of the light incident to the sample, recorded at the position of the sample,the curves represent the absolute reflectivity. The curves are vertically shifted for a bettervisualization of spectrally shifting peaks with the angle of incidence. Measurements whereperformed for angles from = 10 to = 70 in steps of 5 as displayed from bottom totop in Fig. 6.4.

A comparison of the four graphs in Figure 6.4 shows that there is a clear differencein spectra for the different symmetry directions and polarizations. The curves in the

34

Chapter 6. Reflection Experiment 6.4 Experimentally Extracted Q-factors

(a) Sym. polarization TE,direction X

(b) Sym. polarization TE,direction M

(c) Sym. polarization TM,direction X

(d) Sym. polarization TM,direction M

Figure 6.4: Experimental reflectivity data of the PhC for the symmetry directions X and Mand TE and TM polarization. The curves are vertical shifted for clarity, from bottom to top, theangle of incidence increases from = 10 to = 70.

four graphs also show that at these wavelengths the spectra contain many resonances ofdifferent shapes with a weak dependence. The next section gives a closer analysis ofthe individual resonances in the spectra. To retrieve from the observed spectral features,independent of their asymmetry, the center frequency (0) and bandwidth ().

6.4 Experimentally Extracted Q-factors

A closer investigation reveals that the resonances possess different line shapes, such asmaxima, minima, and dispersive (asymmetric) forms. In Section 2.7 the origin of dispersiveline shapes has been explained as interference between light directly (Fresnel) reflected at

35

6.4 Experimentally Extracted Q-factors Chapter 6. Reflection Experiment

the PhC surface and part of the light that first couples to the PhC leaky modes, and thusexperiences a phase shift. The center frequency (0) and width () of these resonances aredirect related with the leaky modes quality factor via Eq. 2.8. Fano functions (Eq. 2.12)are fitted to non overlapping resonances. Two additional fit parameters are required forsuch fits, an offset and a scaling factor, which, however, supposed to leave the retrievedcenter frequency, line width unchanged.

Figure 6.5 shows an example of three Fano fits to demonstrate its suitability to describethe resonances found in the reflectivity curves of Fig. 6.4. All of the graphs contain aselection of the experimental data in which an individual resonance can be identified thathardly shows any overlap with neighbour resonances. Besides the fitted curves, also thefit parameters obtained are displayed in the graphs from which the leaky mode qualityfactor is calculated. During the fit, q is restricted to values between -1 and +1 (compareto Fig. 2.9).

(a) Sym. direction X,polarization TM, = 50

(b) Sym. direction X,polarization TE, = 30

(c) Sym. direction M ,polarization TM, = 60

Figure 6.5: Example of three Fano fits to determine the resonance center frequency and linewidthand calculate the leaky modes quality factor from that. The resonance in (a) has a Q-factor of52.8, in (b) the Q-factor is 54.2 and in (c) a factor of 26.2.

The quality factor is calculated for a total of 225 resonances found in the experimentalreflection data with normalized center frequencies between 0.50.9 (wavelength range 1.11.9 m). In this frequency range higher order modes lie above the designed band gap.

Using the center frequencies obtained by the fits, in Figure 6.6 the dispersion curves ofthe identified leaky modes are constructed in a banddiagram. The center frequencies 0obtained from the Fano fits in combination with the symmetry direction and the incidentangle limits the dots inside the banddiagram to a single position. Dots that belong

36

Chapter 6. Reflection Experiment 6.5 Results and Comparison with Theory

to the same mode are connected with a black line. Within the figure we have chosen

(a) (b)

Figure 6.6: Reconstruction of the leaky modes in a banddiagram.

to add only the measured dispersion curves and not to add any theoretical dispersioncurves. Although it would be possible to fit simulations to the measured curves, we foundit inconvenient due to the high mode density in the measured frequency range.

The distribution of calculated quality factors are displayed in the histograms of Fig-ure 6.7. The histograms 6.7(a,b,d,e) contain the quality factor distribution for the po-larizations and the individual symmetry directions. The histograms 6.7(c,f) only makesa difference in the two polarization states, the symmetry directions are discarded. Thehistograms show that quality factors have values that vary from 17 to 140 for TE modes,and values of 23 to 1500 for TM modes.

6.5 Results and Comparison with Theory

When comparing the calculated intrinsic quality factors (Fig. 5.3) with the measuredquality factors (Fig. 6.7), one notices that the intrinsic quality factors have values from60 to 1800 and that the measured quality factors have values from 17 to 140, and thus arein general lower. This discrepancy between theory and experiment can have two possible

37

6.5 Results and Comparison with Theory Chapter 6. Reflection Experiment

Figure 6.7: Quality factor histograms: (a) TE, X; (b) TE, M ; (c) TE; (d) TM, X;(e) TM, M and (f) TM.

explanations. First, if the spectral resolution of our set-up would habe been to low,it would have limited the contrast of the resonances, which results in broad resonanceswith low quality factors. In our set-up, however, the spectral resolution is limited bythe monochromator to 3.5nm, which gives an estimated quality factor restriction up toQ = 300. Since we have never found quality factors of 300 in our reflection spectra, weknow that this first explanation can not explaining the discrepancy. Second, as describedin Chapter 2.5, we explain the discrepancy to fabrication imperfections which introducesextra (extrinsic) losses.

In order to improve the quality factor, it is advised to search for the most dominantloss factor. For this I recommend extra quality factor studies (simulations) on samples,incorporating one loss mechanism at a time. As LIL provides an excellent periodicity overa large area, I do not expect that hole displacements has a significant influence on thequality factors in our sample. Loss mechanisms from which I expect to have a significantinfluence on the mode quality factors are any cracks from hole to hole and any roughnessinside and on the walls of the holes.

In the next chapter the results of the transmission experiment and the reflection ex-periments are summarized.

38

Chapter 7

Conclusions

We have carried out a linear reflection and transmission experiment on a 2D PhC slab inthe NIR. By comparison to several theoretical models, additional information is gainedon the fabrication quality as can be obtained with a novel type of laser interference litho-graphy for fabricating large area, high contrast 2D Silicon PhCs. The described opticalcharacterization also form the basis for subsequent investigation of third-order nonlineareffects in a 2D PhC slabs, where two-photon absorption is suppressed.

To our knowledge the presented transmission spectra are the first ones obtained froma LIL fabricated 2D PhC slab supported by a waver substrate. Within the transmissionspectra we find sharp resonances superimposed on a Fabry-Perot fringes background.These sharp resonances are the result of interferences between direct transmitted lightand light that first coupled to the PhC leaky modes and diffract out with a certain phasedelay. The Fabry-Perot fringes are formed due to reflections from the planar transparentlayers the PhC consist of.

The measured transmission spectra are compared to a theoretical model to obtain thestructural parameters for our sample. Based on these structure parameters the theoreticalupper limit for the quality factors (intrinsic losses) are predicted for the PhC leaky modes.

In reflection the PhC is investigated for NIR wavelengths. Within the reflection spectraFano-like resonances appear as well, due to coupling of external radiation to the PhCleaky modes. The shape and spectral position of individual resonances are fitted by aFano-function to determine the resonance center frequency and the total Q-factors, whichalso includes extrinsic losses.

The measured quality factors are compared to the theoretically calculated qualityfactors showing that the latter are about 8 times higher. The discrepancies are due tounwanted fabrication imperfections. Those imperfections are the so-called extrinsic losses,such as cracks and roughnesses inside and on the walls of the holes, or the polydispersity

39

Chapter 7. Conclusions

of the hole diameters.

In summary the data presented here are the first measurements of quality for largearea high index PhC slabs. The obtained values for the Q-factors of individual modesshould be of high importance for a realistic judgement of resonant field enhancements insubsequent investigations on optically nonlinear switching effects.

40

Acknowledgements

To all good things comes an end, so does the period in which I was called a student. Duringthis period I met some nice people which I have to express my deepest appreciation to.

First, Id like to thank Klaus Boller for the incredible learning experience he offered mein his group as well for the suggestions for improving this thesis. Petra Gro, Liviu Prodanand Roel Arts, the good help, guidance and suggestions I received on a daily basis wherealways very neat. I couldnt wish myself a better team for this project. Good luck withthe rest of your lives and careers. Id like to thank Kobus Kuipers for his suggestions andanswers about the experiments which made sure I was heading into the right direction.Alfred Schirmacher, thanks for the opportunity you gave us to measure the transmissionof the sample at PTB, all your preparations and help made it a very efficient time. Forthe succeeding of my project I also have to give a major thanks to Peter van der Slot. Hisadvice on one of the last simulations I performed where key for my project. Thanks toHugo Hoekstra to complete my graduation committee.

Traveling an hour by train to my office at the Laser Physics and Nonlinear Opticsgroup wasnt a commitment at all. The people of the group made it always a pleasantarrival for me. The different trips, parties and moments of relaxation by playing cardsduring lunch made it a period I shall not soon forget. Especially the times I made you allloose. Merel, sorry for the bad competition I gave you with websudoku.

The friends I gained from my HTS period are also not to forget. I enjoyed the timewe spend together in and out of school and the vacations we had. Extra thanks to thosewho always offered me a bed on the ground after a night of going out.

My parents and sisters are the one who I give the most credits. There support andencouragements made that I never lost focus to get the best out of myself. Also friendsand family who showed there interest in me,. . . thanks.

Yours,

Enschede, September 2007

41

Bibliography

[1] V. Astratov, I. Culshaw, R. Stevenson, D. Whittaker, M. Skolnick, T. Krauss, andR. de La Rue, Resonant coupling of near-infrared radiation to photonic band struc-ture waveguides, Journal of Lightwave Technology, vol. 17, pp. 2050+, Nov. 1999.

[2] C. Grillet, D. Freeman, B. Luther-Davies, S. Madden, R. McPhedran, D. Moss,M. Steel, and B. Eggleton, Characterization and modeling of Fano resonances inchalcogenide photonic crystal membranes, Optics Express, vol. 14, pp. 369+, Jan.2006.

[3] D. Coquillat, A. Ribayrol, R. de La Rue, M. Le Vassor DYerville, D. Cassagne,and C. Jouanin, First Observations of 2D Photonic Crystal Band Structure inGaN-Sapphire Epitaxial Material, Physica Status Solidi Applied Research, vol. 183,pp. 135138, Feb. 2001.

[4] V. Pacradouni, W. Mandeville, A. Cowan, P. Paddon, J. F. Young, and S. R. John-son, Photonic band structure of dielectric membranes periodically textured in twodimensions, Phys. Rev. B, vol. 62, pp. 42044207, Aug 2000.

[5] A. Cowan, P. Paddon, V. Pacradouni, and J. Young, Resonant scattering and modecoupling in two-dimensional textured planar waveguides, J. Opt. Soc. Am. A, vol. 18,pp. 11601170, 2001.

[6] M. Netti, A. Harris, J. Baumberg, D. Whittaker, M. Charlton, M. Zoorob, andG. Parker, Optical trirefringence in photonic crystal waveguides, Phys. Rev. Lett.,vol. 86, pp. 15261529, Feb 2001.

[7] M. Galli, M. Agio, L. Andreani, L. Atzeni, D. Bajoni, G. Guizzetti, L. Businaro, E. D.Fabrizio, F. Romanato, and A. Passaseo, Optical properties and photonic bands ofgaas photonic crystal waveguides with tilted square lattice, The European PhysicalJournal B - Condensed Matter and Complex Systems, vol. 27, no. 1, pp. 7987, 2002.

[8] K. Crozier, V. Lousse, O. Kilic, S. Kim, S. Fan, and O. Solgaard, Air-bridged pho-tonic crystal slabs at visible and near-infrared wavelengths, Phys. Rev. B, vol. 73,no. 11, p. 115126, 2006.

43

Bibliography

[9] J. Joannopoulos, R. Meade, and J. Winn, Photonic Crystals : Molding the Flow ofLight. Princeton: Princeton University press, 1995.

[10] H. Ibach and H. Luth, Solid-State Physics : An Introduction to Principles of MaterialsScience. Springer, 2nd ed., 1995.

[11] T. Ochiai and K. Sakoda, Nearly free-photon approximation for two-dimensionalphotonic crystal slabs, Phys. Rev. B, vol. 64, p. 045108, Jul 2001.

[12] S. G. Johnson, S. Fan, P. R. Villeneuve, J. Joannopoulos, and L. Kolodziejski,Guided modes in photonic crystal slabs, Phys. Rev. B, vol. 60, pp. 57515758,Aug 1999.

[13] E. Fluck, Local interaction of light with periodic photonic structures. PhD thesis,Optical Techniques Group (OT), Department of Science and Technology, Universityof Twente, 2003.

[14] P. Villeneuve, S. Fan, S. Johnson, and J. Joannopoulos, Three-dimensional photonconfinement in photonic crystals of low-dimensional periodicity, IEE Proceedings -Optoelectronics, vol. 145, no. 6, pp. 384390, 1998.

[15] O. Painter, J. Vuckovic, and A. Scherer, Defect modes of a two-dimensional photoniccrystal in an optically thin dielectric slab, Journal of the Optical Society of AmericaB Optical Physics, vol. 16, pp. 275285, Feb. 1999.

[16] W. Bogaerts, P. Bienstman, D. Taillaert, R. Baets, and D. de Zutter, Out-of-planescattering in 1-D photonic crystal slabs, Optical and Quantum Electronics, vol. 34,pp. 928934, 2002.

[17] S. Fan and J. D. Joannopoulos, Analysis of guided resonances in photonic crystalslabs, Phys. Rev. B, vol. 65, p. 235112, Jun 2002.

[18] S. Johnson. Meep Introduction: http://ab-initio.mit.edu/wiki/index.php/Meep Introduction.

[19] C. Bostan, Design and Fabrication of quasi-2D Photonic Crystal Components basedon SilicononInsulator Technology. PhD thesis, Integrated Optical Microsystems(IOMS), Faculty of Electrical Engineering, Mathematics and Computer Science, Uni-versity of Twente, 2005.

[20] W. Bogaerts, P. Bienstman, and R. Baets, Scattering at sidewall roughness in pho-tonic crystal slabs, Optics Letters, vol. 28, pp. 689691, May 2003.

[21] Y. Tanaka, T. Asano, Y. Akahane, B.-S. Song, and S. Noda, Theoretical investigationof a two-dimensional photonic crystal slab with truncated cone air holes, AppliedPhysics Letters, vol. 82, no. 11, pp. 16611663, 2003.

44

http://ab-initio.mit.edu/wiki/index.php/Meep_Introductionhttp://ab-initio.mit.edu/wiki/index.php/Meep_Introduction

Bibliography

[22] S. Hughes, L. Ramunno, J. F. Young, and J. E. Sipe, Extrinsic optical scatteringloss in photonic crystal waveguides: Role of fabrication disorder and photon groupvelocity, Physical Review Letters, vol. 94, no. 3, p. 033903, 2005.

[23] Diffraction of Water Waves. website: http://www.ngsir.netfirms.com/englishhtm/Diffraction.htm.

[24] U. Fano, Effects of configuration interaction on intensities and phase shifts, Phys.Rev., vol. 124, pp. 18661878, Dec 1961.

[25] Manual DiffractMOD v1.0. website: http://www.rsoftdesign.com/.

[26] J.-P. Berenger, A perfectly matched layer for the absorption of electromagneticwaves, Journal of Computational Physics, vol. 114, pp. 185200, Oct. 1994.

[27] E. Popov, M. Neviere, B. Gralak, and G. Tayeb, Staircase approximation validityfor arbitrary-shaped gratings, J. Opt. Soc. Am. A, vol. 19, pp. 3342, 2002.

[28] S. Johnson and J. Joannopoulos, Block-iterative frequency-domain methods formaxwells equations in a planewave basis, Opt. Express, vol. 8, pp. 173190, Jan.2001.

[29] S. Johnson. MPB Introduction: http://ab-initio.mit.edu/wiki/index.php/MPBIntroduction.

[30] M. Cryan, M. Hill, D. Sanz, P. Ivanov, P. Heard, L. Tian, S. Yu, and J. Rorison, Fo-cused ion beam-based fabrication of nanostructured photonic devices, IEEE Journalof Selected Topics in Quantum Electronics, vol. 11, pp. 12661277, Nov.-Dec. 2005.

[31] T. Krauss, Y. Song, S. Thoms, C. Wilkinson, and R. de la Rue, Fabrication of 2-d photonic bandgap structures in gaas/algaas, Electronics Letters, vol. 30, no. 17,pp. 14441446, 1994.

[32] Y. Vladimirsky, A. Bourdillon, O. Vladimirsky, W. Jiang, and Q. Leonard, Demag-nification in proximity x-ray lithography and extensibility to 25 nm by optimizingfresnel diffraction, Journal of Physics D: Applied Physics, vol. 32, no. 22, pp. L114L118, 1999.

[33] W. Bogaerts, V. Wiaux, D. Taillaert, S. Beckx, B. Luyssaert, P. Bienstman, andR. Baets, Basic structures for photonic integrated circuits in silicon-on-insulator,Optics Express, vol. 12, no. 8, pp. 15831591, 2002.

[34] L. Vogelaar, W. Nijdam, H. van Wolferen, R. de Ridder, F. Segerink, E. Flck,L. Kuipers, and N. van Hulst, Large area photonic crystal slabs for visible lightwith waveguiding defect structures: Fabrication with focused ion beam assisted laserinterference lithography, Adv. Mater., vol. 13, no. 20, pp. 15511554, 2002.

45

http://www.ngsir.netfirms.com/englishhtm/Diffraction.htmhttp://www.ngsir.netfirms.com/englishhtm/Diffraction.htmhttp://www.rsoftdesign.com/http://ab-initio.mit.edu/wiki/index.php/MPB_Introductionhttp://ab-initio.mit.edu/wiki/index.php/MPB_Introduction

Bibliography

[35] L. Prodan, T. Euser, H. Wolferen, C. Bostan, R. Ridder, R. Beigang, K.-J. Boller,and L. Kuipers, Large-area two-dimensional silicon photonic crystals for infraredlight fabricated with laser interference lithography, Nanotechnology, vol. 15, no. 5,pp. 639642, 2004.

[36] Soitec. Parc Technologique des Fontaines, 38190 Bernin, France.website: http://www.soitec.com.

[37] V. Lousse, W. Suh, O. Kilic, O. Solgaard, and S. Fan, Angular and polarizationproperties of a photonic crystal slab mirror, Optics Express, vol. 12, no. 8, 19 April2004.

[38] V. Astratov, M. Skolnick, S. Brand, T. Krauss, O. Karimov, R. Stevenson, D. Whit-taker, I. Culshaw, and R. de La Rue, Experimental technique to determine the bandstructure of two-dimensional photonic lattices, IEE Proc., Optoelectron., vol. 145,pp. 398402, Dec 1998.

46

http://www.soitec.com

Appendix A:

Two-color Characterization of a

2D Photonic Crystal

Poster presented at FOM-meeting Physics @ Veldhoven 2007, 2324 January 2007.

I

PreambleContents1 Introduction2 Theory of Photonic Crystals2.1 Maxwell Equations2.2 Dispersion Relation of a 1D PhC2.3 A 2D Photonic Crystal Slab2.4 Influences on the Dispersion Curves2.5 Quality Factor & Losses2.6 Coupling via Vertical Incidence2.7 Fano Resonances

3 Computational Modeling Tools3.1 RSoft DiffractMOD3.2